#------------------------------------------------------------------------------
#$Date: 2020-11-06 14:21:51 +0200 (Fri, 06 Nov 2020) $
#$Revision: 258859 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/70/53/7705322.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7705322
loop_
_publ_author_name
'Adhikary, Amit'
'Das, Krishna Sundar'
'Saha, Sayan'
'Roy, Manasi'
'Mondal, Raju'
_publ_section_title
;
 A free-standing, self-healing multi-stimuli responsive gel showing
 cryogenic magnetic cooling.
;
_journal_issue                   38
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              13487
_journal_page_last               13495
_journal_paper_doi               10.1039/d0dt02356f
_journal_volume                  49
_journal_year                    2020
_chemical_formula_sum            'C14 H6 Fe2 N2 O13'
_chemical_formula_weight         521.91
_space_group_crystal_system      monoclinic
_space_group_IT_number           15
_space_group_name_Hall           '-C 2yc'
_space_group_name_H-M_alt        'C 1 2/c 1'
_atom_sites_solution_hydrogens   mixed
_audit_block_doi                 10.5517/ccdc.csd.cc20nlx6
_audit_creation_method           SHELXL-2016/6
_audit_update_record
;
2019-03-13 deposited with the CCDC.	2020-08-31 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90.2220(10)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   11.3826(3)
_cell_length_b                   21.6960(9)
_cell_length_c                   7.4517(3)
_cell_measurement_reflns_used    4500
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      30.45
_cell_measurement_theta_min      3.34
_cell_volume                     1840.23(12)
_computing_structure_refinement  'SHELXL-2016/6 (Sheldrick, 2016)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0038
_diffrn_reflns_av_unetI/netI     0.0039
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 1.000
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       28
_diffrn_reflns_limit_k_min       -27
_diffrn_reflns_limit_l_max       9
_diffrn_reflns_limit_l_min       -9
_diffrn_reflns_number            4190
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 1.000
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         27.445
_diffrn_reflns_theta_min         1.877
_exptl_absorpt_coefficient_mu    1.653
_exptl_crystal_colour            Orange
_exptl_crystal_density_diffrn    1.884
_exptl_crystal_description       Block
_exptl_crystal_F_000             1040
_refine_diff_density_max         0.339
_refine_diff_density_min         -0.773
_refine_diff_density_rms         0.056
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.015
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     145
_refine_ls_number_reflns         2102
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.015
_refine_ls_R_factor_all          0.0207
_refine_ls_R_factor_gt           0.0203
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0275P)²+3.1525P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0571
_refine_ls_wR_factor_ref         0.0573
_reflns_Friedel_coverage         0.000
_reflns_number_gt                2060
_reflns_number_total             2102
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            d0dt02356f2.cif
_cod_data_source_block           Complex_1
_cod_depositor_comments          'Adding full bibliography for 7705322.cif.'
_cod_original_sg_symbol_H-M      'C 2/c'
_cod_database_code               7705322
_shelx_shelxl_version_number     2016/6
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y, -z+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y, z-1/2'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Fe1 Fe 0.13211(2) 0.13075(2) 0.79072(3) 0.01933(8) Uani 1 1 d . . . . .
O1 O 0.16525(10) 0.22317(5) 0.81136(14) 0.0219(2) Uani 1 1 d . . . . .
O2 O 0.28688(11) 0.30044(5) 0.73417(15) 0.0265(2) Uani 1 1 d . . . . .
O3 O 0.18356(9) 0.04187(5) 0.71712(16) 0.0246(2) Uani 1 1 d . . . . .
O4 O 0.32612(10) -0.01474(5) 0.59165(18) 0.0299(3) Uani 1 1 d . . . . .
O5 O 0.21282(11) 0.11443(5) 1.02486(15) 0.0267(2) Uani 1 1 d . . . . .
H5A H 0.172298 0.129624 1.109795 0.040 Uiso 1 1 d R U . . .
H5B H 0.277315 0.134226 1.028749 0.040 Uiso 1 1 d R U . . .
O6 O 0.02074(9) 0.13236(5) 0.58704(15) 0.0227(2) Uani 1 1 d . . . . .
N1 N 0.28941(10) 0.14282(5) 0.65759(16) 0.0164(2) Uani 1 1 d . . . . .
C1 C 0.33280(12) 0.19938(6) 0.64275(19) 0.0172(3) Uani 1 1 d . . . . .
C2 C 0.43618(13) 0.21025(7) 0.5523(2) 0.0224(3) Uani 1 1 d . . . . .
H2 H 0.465611 0.249988 0.539406 0.027 Uiso 1 1 calc R U . . .
C3 C 0.49479(13) 0.15980(8) 0.4812(2) 0.0235(3) Uani 1 1 d . . . . .
H3 H 0.564365 0.165717 0.418459 0.028 Uiso 1 1 calc R U . . .
C4 C 0.45045(12) 0.10024(7) 0.5028(2) 0.0219(3) Uani 1 1 d . . . . .
H4 H 0.490160 0.066134 0.457867 0.026 Uiso 1 1 calc R U . . .
C5 C 0.34582(12) 0.09385(6) 0.59294(19) 0.0180(3) Uani 1 1 d . . . . .
C6 C 0.25706(13) 0.24572(6) 0.73611(19) 0.0195(3) Uani 1 1 d . . . . .
C7 C 0.28113(12) 0.03479(7) 0.6357(2) 0.0211(3) Uani 1 1 d . . . . .
O13 O 1.000000 0.05800(11) 0.250000 0.0519(5) Uani 1 2 d GS T P . .
H13 H 0.942341 0.082827 0.243912 0.078 Uiso 0.5 1 d G U P . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Fe Fe 0.3463 0.8444 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_citation_id
_citation_doi
_citation_year
1 10.1021/acsomega.8b03400 2019
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O6 Fe1 O6 77.83(5) 2_556 . ?
O6 Fe1 O5 90.19(5) 2_556 . ?
O6 Fe1 O5 164.84(5) . . ?
O6 Fe1 O1 96.37(4) 2_556 . ?
O6 Fe1 O1 99.10(4) . . ?
O5 Fe1 O1 91.37(5) . . ?
O6 Fe1 N1 171.59(5) 2_556 . ?
O6 Fe1 N1 100.58(5) . . ?
O5 Fe1 N1 92.59(5) . . ?
O1 Fe1 N1 75.64(4) . . ?
O6 Fe1 O3 112.78(4) 2_556 . ?
O6 Fe1 O3 89.68(5) . . ?
O5 Fe1 O3 86.41(5) . . ?
O1 Fe1 O3 150.75(4) . . ?
N1 Fe1 O3 75.33(4) . . ?
C6 O1 Fe1 119.37(9) . . ?
C7 O3 Fe1 118.74(9) . . ?
Fe1 O5 H5A 109.4 . . ?
Fe1 O5 H5B 109.5 . . ?
H5A O5 H5B 104.4 . . ?
Fe1 O6 Fe1 102.13(5) 2_556 . ?
C1 N1 C5 121.80(12) . . ?
C1 N1 Fe1 118.71(10) . . ?
C5 N1 Fe1 119.47(9) . . ?
N1 C1 C2 121.16(13) . . ?
N1 C1 C6 111.52(12) . . ?
C2 C1 C6 127.31(13) . . ?
C1 C2 C3 117.65(13) . . ?
C1 C2 H2 121.2 . . ?
C3 C2 H2 121.2 . . ?
C2 C3 C4 120.74(14) . . ?
C2 C3 H3 119.6 . . ?
C4 C3 H3 119.6 . . ?
C5 C4 C3 117.58(14) . . ?
C5 C4 H4 121.2 . . ?
C3 C4 H4 121.2 . . ?
N1 C5 C4 121.01(13) . . ?
N1 C5 C7 111.32(12) . . ?
C4 C5 C7 127.66(13) . . ?
O2 C6 O1 126.53(14) . . ?
O2 C6 C1 118.77(14) . . ?
O1 C6 C1 114.69(12) . . ?
O4 C7 O3 126.38(14) . . ?
O4 C7 C5 118.57(13) . . ?
O3 C7 C5 115.05(12) . . ?
H13 O13 H13 101.4 . 2_755 ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Fe1 O6 1.9673(11) 2_556 ?
Fe1 O6 1.9740(12) . ?
Fe1 O5 2.0003(12) . ?
Fe1 O1 2.0459(10) . ?
Fe1 N1 2.0669(12) . ?
Fe1 O3 2.0893(10) . ?
O1 C6 1.2847(19) . ?
O2 C6 1.2350(18) . ?
O3 C7 1.2767(17) . ?
O4 C7 1.2354(18) . ?
O5 H5A 0.8510 . ?
O5 H5B 0.8509 . ?
N1 C1 1.3275(17) . ?
N1 C5 1.3325(18) . ?
C1 C2 1.379(2) . ?
C1 C6 1.498(2) . ?
C2 C3 1.388(2) . ?
C2 H2 0.9300 . ?
C3 C4 1.397(2) . ?
C3 H3 0.9300 . ?
C4 C5 1.3767(19) . ?
C4 H4 0.9300 . ?
C5 C7 1.5124(19) . ?
O13 H13 0.8501 . ?
O13 H13 0.85(6) 2_755 ?
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
C5 N1 C1 C2 2.9(2) . . . . ?
Fe1 N1 C1 C2 -178.71(10) . . . . ?
C5 N1 C1 C6 -176.32(12) . . . . ?
Fe1 N1 C1 C6 2.06(15) . . . . ?
N1 C1 C2 C3 -1.6(2) . . . . ?
C6 C1 C2 C3 177.53(13) . . . . ?
C1 C2 C3 C4 -0.6(2) . . . . ?
C2 C3 C4 C5 1.5(2) . . . . ?
C1 N1 C5 C4 -2.0(2) . . . . ?
Fe1 N1 C5 C4 179.66(11) . . . . ?
C1 N1 C5 C7 177.01(13) . . . . ?
Fe1 N1 C5 C7 -1.36(16) . . . . ?
C3 C4 C5 N1 -0.2(2) . . . . ?
C3 C4 C5 C7 -179.03(14) . . . . ?
Fe1 O1 C6 O2 178.43(11) . . . . ?
Fe1 O1 C6 C1 -1.46(16) . . . . ?
N1 C1 C6 O2 179.70(13) . . . . ?
C2 C1 C6 O2 0.5(2) . . . . ?
N1 C1 C6 O1 -0.40(17) . . . . ?
C2 C1 C6 O1 -179.58(13) . . . . ?
Fe1 O3 C7 O4 176.19(13) . . . . ?
Fe1 O3 C7 C5 -3.22(18) . . . . ?
N1 C5 C7 O4 -176.52(14) . . . . ?
C4 C5 C7 O4 2.4(2) . . . . ?
N1 C5 C7 O3 2.94(19) . . . . ?
C4 C5 C7 O3 -178.17(15) . . . . ?
